#------------------------------------------------------------------------------
#$Date: 2016-03-22 10:37:57 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178878 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/07/4110715.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4110715
loop_
_publ_author_name
'Kazunari Yamaura'
'Qingzhen Huang'
'Lianqi Zhang'
'Kazunori Takada'
'Yuji Baba'
'Takuro Nagai'
'Yoshio Matsui'
'Kosuke Kosuda'
'Eiji Takayama-Muromachi'
_publ_section_title
;
 Spinel-to-CaFe2O4-Type Structural Transformation in LiMn2O4 under High
 Pressure
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              9448
_journal_page_last               9456
_journal_paper_doi               10.1021/ja0612302
_journal_volume                  128
_journal_year                    2006
_chemical_formula_sum            'Li0.46 Mn O2'
_chemical_formula_weight         90.12
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            8
_cell_length_a                   8.8336(5)
_cell_length_b                   2.83387(18)
_cell_length_c                   10.6535(7)
_cell_volume                     266.69(3)
_pd_phase_name                   Li0.92Mn2O4
_cod_data_source_file            ja0612302si20060302_021812.cif
_cod_data_source_block           Li0.92Mn2O4
_cod_depositor_comments          'Adding Fobs data.'
_cod_original_cell_volume        266.691(29)
_cod_database_code               4110715
_cod_database_fobs_code          4110715
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -x+1/2,+y+1/2,+z+1/2
3 +x,-y+1/2,+z
4 -x+1/2,-y,+z+1/2
-1 -x,-y,-z
-2 +x+1/2,-y+1/2,-z+1/2
-3 -x,+y+1/2,-z
-4 +x+1/2,+y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Li Li 0.278(4) 0.25 0.370(4) 0.91667 Uiso 0.127(14) 4
Mn Mn1 0.0584(10) 0.25 0.1188(8) 1.0 Uiso 0.0349(22) 4
Mn Mn2 0.0828(8) 0.25 0.6082(6) 1.0 Uiso 0.0146(14) 4
O O1 0.3061(6) 0.25 0.6508(6) 1.0 Uiso 0.0343(12) 4
O O2 0.3801(9) 0.25 0.9799(6) 1.0 Uiso 0.0628(20) 4
O O3 0.4764(8) 0.25 0.2072(6) 1.0 Uiso 0.0515(18) 4
O O4 0.0707(8) 0.25 0.9269(6) 1.0 Uiso 0.0535(19) 4
loop_
_atom_type_symbol
_atom_type_number_in_cell
Li 3.667
Mn 8.0
O 16.0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Li Li Li 180.0 1_545 1_565 n
Li Li Mn1 90.00000(20) 1_545 -2_656 n
Li Li O2 52.2(6) 1_545 2_544 n
Li Li O2 127.8(6) 1_545 2_554 n
Li Li O4 46.0(8) 1_545 2_544 n
Li Li O4 134.0(8) 1_545 2_554 n
Li Li Mn1 90.00000(20) 1_565 -2_656 n
Li Li O2 127.8(6) 1_565 2_544 n
Li Li O2 52.2(6) 1_565 2_554 n
Li Li O4 134.0(8) 1_565 2_544 n
Li Li O4 46.0(8) 1_565 2_554 n
Mn1 Li O2 125.4(13) -2_666 2_544 n
Mn1 Li O2 125.4(13) -2_666 2_554 n
Mn1 Li O4 48.1(8) -2_666 2_544 n
Mn1 Li O4 48.1(8) -2_666 2_554 n
O2 Li O2 75.5(11) 2_544 2_554 n
O2 Li O4 79.5(7) 2_544 2_544 n
O2 Li O4 132.0(19) 2_544 2_554 n
O2 Li O4 132.0(19) 2_554 2_544 n
O2 Li O4 79.5(7) 2_554 2_554 n
O4 Li O4 88.1(16) 2_544 2_554 n
Li Mn1 O1 128.67(35) -2_566 2_544 n
Li Mn1 O1 128.67(35) -2_566 2_554 n
Li Mn1 O3 65.8(9) -2_566 -2_566 n
Li Mn1 O4 95.9(9) -2_566 1_554 n
Li Mn1 O4 53.7(4) -2_566 -1_556 n
Li Mn1 O4 53.7(4) -2_566 -1_566 n
O1 Mn1 O1 97.4(5) 2_544 2_554 n
O1 Mn1 O3 93.6(4) 2_544 -2_566 n
O1 Mn1 O4 98.4(4) 2_544 1_554 n
O1 Mn1 O4 82.27(18) 2_544 -1_556 n
O1 Mn1 O4 175.2(6) 2_544 -1_566 n
O1 Mn1 O3 93.6(4) 2_554 -2_566 n
O1 Mn1 O4 98.4(4) 2_554 1_554 n
O1 Mn1 O4 175.2(6) 2_554 -1_556 n
O1 Mn1 O4 82.27(18) 2_554 -1_566 n
O3 Mn1 O4 161.7(6) -2_566 1_554 n
O3 Mn1 O4 91.2(4) -2_566 -1_556 n
O3 Mn1 O4 91.2(4) -2_566 -1_566 n
O4 Mn1 O4 76.9(4) 1_554 -1_556 n
O4 Mn1 O4 76.9(4) 1_554 -1_566 n
O4 Mn1 O4 97.6(5) -1_556 -1_566 n
O1 Mn2 O2 89.63(32) 1_555 2_544 n
O1 Mn2 O2 89.63(32) 1_555 2_554 n
O1 Mn2 O2 165.3(4) 1_555 -2_567 n
O1 Mn2 O3 98.52(34) 1_555 2_545 n
O1 Mn2 O3 98.52(34) 1_555 2_555 n
O2 Mn2 O2 90.5(4) 2_544 2_554 n
O2 Mn2 O2 80.07(35) 2_544 -2_567 n
O2 Mn2 O3 83.82(19) 2_544 2_545 n
O2 Mn2 O3 170.0(5) 2_544 2_555 n
O2 Mn2 O2 80.07(35) 2_554 -2_567 n
O2 Mn2 O3 170.0(5) 2_554 2_545 n
O2 Mn2 O3 83.82(19) 2_554 2_555 n
O2 Mn2 O3 90.8(4) -2_567 2_545 n
O2 Mn2 O3 90.8(4) -2_567 2_555 n
O3 Mn2 O3 100.6(5) 2_545 2_555 n
Mn1 O1 Mn1 97.4(5) 2_545 2_555 n
Mn1 O1 Mn2 125.30(28) 2_545 1_555 n
Mn1 O1 Mn2 125.30(28) 2_555 1_555 n
Li O2 Li 75.5(11) 2_545 2_555 n
Li O2 Mn2 90.7(7) 2_545 2_545 n
Li O2 Mn2 151.9(10) 2_545 2_555 n
Li O2 Mn2 107.5(10) 2_545 -2_566 n
Li O2 Mn2 151.9(10) 2_555 2_545 n
Li O2 Mn2 90.7(7) 2_555 2_555 n
Li O2 Mn2 107.5(10) 2_555 -2_566 n
Mn2 O2 Mn2 90.5(4) 2_545 2_555 n
Mn2 O2 Mn2 99.93(35) 2_545 -2_566 n
Mn2 O2 Mn2 99.93(35) 2_555 -2_566 n
Mn1 O3 Mn2 129.53(23) -2_565 2_544 n
Mn1 O3 Mn2 129.53(23) -2_565 2_554 n
Mn2 O3 Mn2 100.6(5) 2_544 2_554 n
Li O4 Li 88.1(16) 2_545 2_555 n
Li O4 Mn1 109.5(11) 2_545 1_556 n
Li O4 Mn1 78.2(9) 2_545 -1_556 n
Li O4 Mn1 147.3(11) 2_545 -1_566 n
Li O4 Mn1 109.5(11) 2_555 1_556 n
Li O4 Mn1 147.3(11) 2_555 -1_556 n
Li O4 Mn1 78.2(9) 2_555 -1_566 n
Mn1 O4 Mn1 103.1(4) 1_556 -1_556 n
Mn1 O4 Mn1 103.1(4) 1_556 -1_566 n
Mn1 O4 Mn1 97.6(5) -1_556 -1_566 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Li Li 2.83387(18) 1_545 n
Li Li 2.83387(18) 1_565 n
Li Mn1 2.48(4) -2_555 n
Li Mn2 3.07(4) 1_555 n
Li O1 2.829(33) 2_544 n
Li O1 2.829(33) 2_554 n
Li O2 2.313(30) 2_544 n
Li O2 2.313(30) 2_554 n
Li O3 2.46(4) 1_555 n
Li O3 2.79(4) -2_455 n
Li O4 2.038(30) 2_544 n
Li O4 2.038(30) 2_554 n
Mn1 Li 2.48(4) -2_455 n
Mn1 Mn1 2.83387(18) 1_545 n
Mn1 Mn1 2.83387(18) 1_565 n
Mn1 O1 1.886(7) 2_544 n
Mn1 O1 1.886(7) 2_554 n
Mn1 O3 1.991(11) -2_455 n
Mn1 O4 2.047(10) 1_554 n
Mn1 O4 1.883(7) -1_556 n
Mn1 O4 1.883(7) -1_566 n
Mn2 Li 3.07(4) 1_555 n
Mn2 Mn2 2.83387(18) 1_545 n
Mn2 Mn2 2.83387(18) 1_565 n
Mn2 O1 2.025(9) 1_555 n
Mn2 O2 1.995(7) 2_544 n
Mn2 O2 1.995(7) 2_554 n
Mn2 O2 2.021(11) -2_456 n
Mn2 O3 1.842(6) 2_545 n
Mn2 O3 1.842(6) 2_555 n
O1 Li 2.829(33) 2_545 n
O1 Li 2.829(33) 2_555 n
O1 Mn1 1.886(7) 2_545 n
O1 Mn1 1.886(7) 2_555 n
O1 Mn2 2.025(9) 1_555 n
O2 Li 2.313(30) 2_545 n
O2 Li 2.313(30) 2_555 n
O2 Mn2 1.995(7) 2_545 n
O2 Mn2 1.995(7) 2_555 n
O2 Mn2 2.021(11) -2_556 n
O3 Li 2.46(4) 1_555 n
O3 Li 2.79(4) -2_555 n
O3 Mn1 1.991(11) -2_555 n
O3 Mn2 1.842(6) 2_544 n
O3 Mn2 1.842(6) 2_554 n
O4 Li 2.038(30) 2_545 n
O4 Li 2.038(30) 2_555 n
O4 Mn1 2.047(10) 1_556 n
O4 Mn1 1.883(7) -1_556 n
O4 Mn1 1.883(7) -1_566 n
